#------------------------------------------------------------------------------
#$Date: 2017-04-11 08:10:29 +0300 (Tue, 11 Apr 2017) $
#$Revision: 195328 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/22/80/7228052.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7228052
loop_
_publ_author_name
'Guo, Li-Ying'
'Li, Ying'
'Zhang, Yao'
'Li, Jian-Sheng'
'You, Wan-Sheng'
'Su, Fang'
'Zhu, Zai-Ming'
'Sang, Xiao-Jing'
'Zhang, Lan-Cui'
_publ_section_title
;
 Extended visible photosensitivity of carboxyethyltin functionalized
 polyoxometalates with common organic dyes enabling enhanced photoelectric
 performance
;
_journal_issue                   33
_journal_name_full               'RSC Adv.'
_journal_page_first              20685
_journal_paper_doi               10.1039/C7RA02353G
_journal_volume                  7
_journal_year                    2017
_chemical_formula_moiety         'C18 H84 Cu2 N36 O116 P4 Sn2 W30,14H2O'
_chemical_formula_sum            'C18 H112 Cu2 N36 O130 P4 Sn2 W30'
_chemical_formula_weight         8917.27
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2yn'
_space_group_name_H-M_alt        'P 1 21/n 1'
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2014/7
_audit_update_record
;
2017-03-30 deposited with the CCDC.
2017-04-05 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 94.0540(10)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   13.3227(7)
_cell_length_b                   32.2012(16)
_cell_length_c                   19.0960(10)
_cell_measurement_reflns_used    6318
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      28.72
_cell_measurement_theta_min      1.81
_cell_volume                     8171.8(7)
_computing_cell_refinement       'SMART (Bruker, 2005)'
_computing_data_collection       'SMART (Bruker, 2005)'
_computing_data_reduction        SAINT
_computing_molecular_graphics    'SHELXTL (Sheldrick, 1997a)'
_computing_publication_material  SHELXTL
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1997b)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0771
_diffrn_reflns_av_unetI/netI     0.0896
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.999
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_k_max       34
_diffrn_reflns_limit_k_min       -38
_diffrn_reflns_limit_l_max       22
_diffrn_reflns_limit_l_min       -21
_diffrn_reflns_number            42009
_diffrn_reflns_point_group_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.999
_diffrn_reflns_theta_full        24.999
_diffrn_reflns_theta_max         24.999
_diffrn_reflns_theta_min         1.805
_diffrn_source                   'fine-focus sealed tube'
_exptl_absorpt_coefficient_mu    21.719
_exptl_absorpt_correction_T_max  0.3980
_exptl_absorpt_correction_T_min  0.2296
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   '(SADABS; Sheldrick, 2003)'
_exptl_crystal_colour            light-green
_exptl_crystal_density_diffrn    3.624
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             7900
_exptl_crystal_size_max          0.096
_exptl_crystal_size_mid          0.067
_exptl_crystal_size_min          0.052
_platon_squeeze_details
;
;
_refine_diff_density_max         2.144
_refine_diff_density_min         -2.894
_refine_diff_density_rms         0.371
_refine_ls_extinction_coef       0.000017(5)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2014/7 (Sheldrick 2014'
_refine_ls_goodness_of_fit_ref   1.015
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     954
_refine_ls_number_reflns         14381
_refine_ls_number_restraints     166
_refine_ls_restrained_S_all      1.019
_refine_ls_R_factor_all          0.0936
_refine_ls_R_factor_gt           0.0501
_refine_ls_shift/su_max          0.004
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0443P)²+195.0548P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1083
_refine_ls_wR_factor_ref         0.1264
_reflns_Friedel_coverage         0.000
_reflns_number_gt                9488
_reflns_number_total             14381
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            c7ra02353g2.cif
_cod_data_source_block           SnR-Cu-P2W15
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_absorpt_correction_type' value 'Multi-scan' changed to
'multi-scan' according to
/home/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 4973 2017-02-22 13:04:09Z antanas 
;
_cod_database_code               7228052
_shelx_shelxl_version_number     2014/7
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_min   0.230
_shelx_estimated_absorpt_t_max   0.398
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, -y-1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
W1 W 0.33361(6) 0.10130(2) 0.42308(4) 0.01894(19) Uani 1 1 d . . .
W2 W 0.55892(6) 0.17387(3) 0.79922(5) 0.0234(2) Uani 1 1 d . . .
W3 W 0.30821(6) 0.16189(3) 0.77837(4) 0.0230(2) Uani 1 1 d . . .
W4 W 0.21165(6) 0.06434(3) 0.55927(4) 0.0241(2) Uani 1 1 d . . .
W5 W 0.61398(6) 0.11513(2) 0.44552(4) 0.01861(19) Uani 1 1 d . . .
W6 W 0.17481(6) 0.17912(3) 0.60478(5) 0.0223(2) Uani 1 1 d . . .
W7 W 0.57336(6) 0.22711(3) 0.49190(5) 0.0230(2) Uani 1 1 d . . .
W8 W 0.59588(6) 0.06107(3) 0.75150(4) 0.0208(2) Uani 1 1 d . . .
W9 W 0.69794(6) 0.20425(3) 0.64685(5) 0.0250(2) Uani 1 1 d . . .
W10 W 0.73461(6) 0.09041(3) 0.60124(5) 0.0280(2) Uani 1 1 d . . .
W11 W 0.30109(6) 0.21374(3) 0.46985(5) 0.0226(2) Uani 1 1 d . . .
W12 W 0.34505(6) 0.04903(3) 0.73127(4) 0.0206(2) Uani 1 1 d . . .
W13 W 0.40821(7) 0.30279(3) 0.57344(5) 0.0282(2) Uani 1 1 d . . .
W14 W 0.53500(6) 0.28147(3) 0.72903(5) 0.0271(2) Uani 1 1 d . . .
W15 W 0.27873(6) 0.26932(3) 0.70903(5) 0.0264(2) Uani 1 1 d . . .
Sn1 Sn 0.49906(10) -0.02763(4) 0.64837(7) 0.0220(3) Uani 1 1 d . U .
Cu1 Cu 0.37709(18) -0.00667(8) 0.49073(13) 0.0252(6) Uani 1 1 d . . .
P1 P 0.4746(3) 0.07344(15) 0.5830(3) 0.0140(10) Uani 1 1 d . . .
P2 P 0.4351(3) 0.19725(15) 0.6332(3) 0.0151(11) Uani 1 1 d . . .
O1 O 0.0862(10) 0.0542(5) 0.5607(7) 0.029(3) Uani 1 1 d . . .
O2 O 0.6843(10) 0.0872(4) 0.6900(7) 0.024(3) Uani 1 1 d . . .
O3 O 0.3761(9) 0.0023(4) 0.6837(6) 0.021(3) Uani 1 1 d . . .
O4 O 0.3039(10) 0.1547(4) 0.4496(7) 0.026(3) Uani 1 1 d . . .
O5 O 0.4683(9) 0.0774(4) 0.6619(6) 0.019(3) Uani 1 1 d . . .
O6 O 0.4737(9) 0.1141(4) 0.4211(7) 0.019(3) Uani 1 1 d . . .
O7 O 0.2233(10) 0.1589(5) 0.8422(8) 0.036(4) Uani 1 1 d . . .
O8 O 0.5629(10) 0.1185(4) 0.7820(7) 0.025(3) Uani 1 1 d . . .
O9 O 0.2198(10) 0.1614(4) 0.6947(7) 0.024(3) Uani 1 1 d . . .
O10 O 0.6535(10) 0.1832(4) 0.7298(7) 0.028(3) Uani 1 1 d . . .
O11 O 0.2184(9) 0.0788(4) 0.4598(6) 0.017(3) Uani 1 1 d . . .
O12 O 0.4691(10) 0.0472(4) 0.7880(7) 0.026(3) Uani 1 1 d . . .
O13 O 0.6629(9) 0.1213(4) 0.3661(7) 0.027(3) Uani 1 1 d . . .
O14 O 0.4365(9) 0.1728(4) 0.7014(7) 0.020(3) Uani 1 1 d . . .
O15 O 0.7305(9) 0.1029(4) 0.5005(7) 0.022(3) Uani 1 1 d . . .
O16 O 0.5654(9) 0.0957(4) 0.5574(6) 0.021(3) Uani 1 1 d . . .
O17 O 0.3762(9) 0.0876(4) 0.5425(7) 0.022(3) Uani 1 1 d . . .
O18 O 0.2054(9) 0.2359(4) 0.6446(7) 0.023(3) Uani 1 1 d . . .
O19 O 0.3368(10) 0.1074(4) 0.7641(7) 0.025(3) Uani 1 1 d . . .
O20 O 0.5348(9) 0.1949(4) 0.5976(7) 0.021(3) Uani 1 1 d . . .
O21 O 0.7160(9) 0.1523(4) 0.6100(7) 0.024(3) Uani 1 1 d . . .
O22 O 0.3006(11) 0.2233(4) 0.7667(7) 0.032(4) Uani 1 1 d . . .
O23 O 0.6077(10) 0.1694(4) 0.4745(7) 0.025(3) Uani 1 1 d . U .
O24 O 0.6206(10) 0.2478(4) 0.4185(8) 0.032(4) Uani 1 1 d . . .
O25 O 0.2929(10) 0.1051(4) 0.3369(7) 0.031(4) Uani 1 1 d . . .
O26 O 0.3453(9) 0.1853(4) 0.5835(8) 0.026(3) Uani 1 1 d . . .
O27 O 0.4888(11) 0.0245(4) 0.5667(7) 0.032(4) Uani 1 1 d . . .
O28 O 0.2633(10) 0.0299(4) 0.7864(7) 0.030(4) Uani 1 1 d . . .
O29 O 0.8182(10) 0.2182(5) 0.6731(7) 0.033(4) Uani 1 1 d . . .
O30 O 0.1794(9) 0.2057(4) 0.5131(7) 0.026(3) Uani 1 1 d . . .
O31 O 0.3989(12) 0.3469(4) 0.5242(10) 0.049(5) Uani 1 1 d . . .
O32 O 0.1873(11) 0.2960(4) 0.7479(8) 0.037(4) Uani 1 1 d . . .
O33 O 0.6029(11) 0.3173(4) 0.7805(9) 0.039(4) Uani 1 1 d . . .
O34 O 0.4408(9) 0.2113(4) 0.4586(7) 0.021(3) Uani 1 1 d . . .
O35 O 0.5954(10) 0.0136(4) 0.7016(7) 0.022(3) Uani 1 1 d . . .
O36 O 0.5174(9) 0.2738(4) 0.5303(7) 0.024(3) Uani 1 1 d . . .
O37 O 0.3256(10) 0.2648(4) 0.5147(7) 0.028(3) Uani 1 1 d . . .
O38 O 0.8619(10) 0.0908(5) 0.6215(7) 0.032(4) Uani 1 1 d . . .
O39 O 0.3856(9) 0.0407(4) 0.4145(7) 0.021(3) Uani 1 1 d . . .
O40 O 0.2634(10) 0.0138(5) 0.5449(7) 0.034(4) Uani 1 1 d . . .
O41 O 0.6930(9) 0.2299(4) 0.5544(7) 0.023(3) Uani 1 1 d . . .
O42 O 0.3999(10) 0.2946(4) 0.7544(7) 0.031(4) Uani 1 1 d . . .
O43 O 0.5321(10) 0.2349(4) 0.7855(7) 0.029(3) Uani 1 1 d . . .
O44 O 0.0477(10) 0.1820(4) 0.6110(7) 0.026(3) Uani 1 1 d . . .
O45 O 0.6323(9) 0.2567(4) 0.6793(7) 0.024(3) Uani 1 1 d . . .
O46 O 0.6748(10) 0.0484(4) 0.8224(7) 0.030(4) Uani 1 1 d . . .
O47 O 0.2513(9) 0.0670(4) 0.6557(7) 0.021(3) Uani 1 1 d . . .
O48 O 0.2534(11) 0.2299(4) 0.3905(7) 0.031(4) Uani 1 1 d . . .
O49 O 0.6341(11) 0.1781(4) 0.8758(8) 0.033(4) Uani 1 1 d . . .
O50 O 0.1881(9) 0.1274(4) 0.5693(7) 0.020(3) Uani 1 1 d . . .
O51 O 0.4299(10) 0.1714(4) 0.8358(7) 0.028(3) Uani 1 1 d . . .
O52 O 0.5966(10) 0.0515(4) 0.4314(7) 0.021(3) Uani 1 1 d . . .
O53 O 0.4199(9) 0.2449(4) 0.6523(7) 0.021(3) Uani 1 1 d . . .
O54 O 0.5033(10) 0.3177(4) 0.6468(7) 0.030(4) Uani 1 1 d . . .
O55 O 0.7158(10) 0.0362(4) 0.5811(7) 0.031(4) Uani 1 1 d . . .
O56 O 0.3002(10) 0.3073(5) 0.6309(7) 0.034(4) Uani 1 1 d . . .
O57 O 0.4052(19) -0.1158(8) 0.8571(14) 0.116(5) Uani 1 1 d D U .
O58 O 0.5715(19) -0.0962(8) 0.8861(14) 0.114(5) Uani 1 1 d D U .
N1 N -0.0552(14) -0.1307(6) 0.6038(11) 0.048(5) Uani 1 1 d . U .
H1C H -0.1030 -0.1192 0.5782 0.058 Uiso 1 1 calc R U .
H1D H -0.0690 -0.1469 0.6376 0.058 Uiso 1 1 calc R U .
N2 N 0.0629(15) -0.0991(6) 0.5404(11) 0.051(6) Uani 1 1 d . U .
H2C H 0.0162 -0.0872 0.5142 0.062 Uiso 1 1 calc R U .
H2D H 0.1250 -0.0948 0.5331 0.062 Uiso 1 1 calc R U .
N3 N 0.1116(14) -0.1410(6) 0.6341(11) 0.057(7) Uani 1 1 d . . .
H3A H 0.1739 -0.1362 0.6282 0.068 Uiso 1 1 calc R U .
H3B H 0.0955 -0.1571 0.6675 0.068 Uiso 1 1 calc R U .
N4 N 0.0060(14) 0.2355(7) 0.4352(11) 0.055(6) Uani 1 1 d . . .
H4A H 0.0212 0.2458 0.3959 0.066 Uiso 1 1 calc R U .
H4B H 0.0526 0.2261 0.4645 0.066 Uiso 1 1 calc R U .
N5 N -0.1581(16) 0.2473(8) 0.4091(13) 0.081(9) Uani 1 1 d . . .
H5A H -0.1459 0.2579 0.3692 0.098 Uiso 1 1 calc R U .
H5B H -0.2190 0.2458 0.4211 0.098 Uiso 1 1 calc R U .
N6 N -0.1030(17) 0.2178(7) 0.5124(12) 0.062(6) Uani 1 1 d . U .
H6A H -0.1635 0.2163 0.5253 0.074 Uiso 1 1 calc R U .
H6B H -0.0536 0.2089 0.5397 0.074 Uiso 1 1 calc R U .
N7 N 0.998(2) 0.1889(9) 0.7748(15) 0.092(10) Uani 1 1 d . . .
H7A H 0.9638 0.1992 0.7392 0.110 Uiso 1 1 calc R U .
H7B H 1.0617 0.1843 0.7726 0.110 Uiso 1 1 calc R U .
N8 N 0.862(2) 0.1863(12) 0.8371(19) 0.135(15) Uani 1 1 d . . .
H8A H 0.8342 0.1806 0.8751 0.162 Uiso 1 1 calc R U .
H8B H 0.8271 0.1964 0.8016 0.162 Uiso 1 1 calc R U .
N9 N 1.0078(17) 0.1648(7) 0.8857(14) 0.068(7) Uani 1 1 d . . .
H9A H 0.9808 0.1589 0.9241 0.082 Uiso 1 1 calc R U .
H9B H 1.0710 0.1605 0.8823 0.082 Uiso 1 1 calc R U .
N10 N 0.9095(16) 0.0784(9) 0.7815(13) 0.078(8) Uani 1 1 d . . .
H10A H 0.8842 0.0738 0.8210 0.094 Uiso 1 1 calc R U .
H10B H 0.8714 0.0864 0.7458 0.094 Uiso 1 1 calc R U .
N11 N 1.0440(17) 0.0818(9) 0.7151(11) 0.078(9) Uani 1 1 d . . .
H11A H 1.1075 0.0795 0.7105 0.093 Uiso 1 1 calc R U .
H11B H 1.0044 0.0897 0.6802 0.093 Uiso 1 1 calc R U .
N12 N 1.064(2) 0.0613(9) 0.8301(16) 0.104(10) Uani 1 1 d . U .
H12A H 1.1282 0.0587 0.8272 0.124 Uiso 1 1 calc R U .
H12B H 1.0382 0.0560 0.8690 0.124 Uiso 1 1 calc R U .
N13 N 0.3250(18) 0.1951(8) 0.2507(13) 0.071(7) Uani 1 1 d . U .
H13A H 0.2996 0.1943 0.2908 0.085 Uiso 1 1 calc R U .
H13B H 0.2861 0.1963 0.2128 0.085 Uiso 1 1 calc R U .
N14 N 0.4843(17) 0.1926(9) 0.3040(12) 0.081(9) Uani 1 1 d . . .
H14A H 0.5482 0.1960 0.3030 0.097 Uiso 1 1 calc R U .
H14B H 0.4584 0.1881 0.3433 0.097 Uiso 1 1 calc R U .
N15 N 0.462(3) 0.2013(10) 0.1841(17) 0.117(11) Uani 1 1 d . U .
H15A H 0.5250 0.2049 0.1801 0.140 Uiso 1 1 calc R U .
H15B H 0.4204 0.2022 0.1474 0.140 Uiso 1 1 calc R U .
N16 N 0.179(2) 0.0196(8) 0.2993(14) 0.082(7) Uani 1 1 d . U .
H16A H 0.2304 0.0097 0.3234 0.098 Uiso 1 1 calc R U .
H16B H 0.1857 0.0298 0.2582 0.098 Uiso 1 1 calc R U .
N17 N 0.073(2) 0.0037(9) 0.3896(16) 0.097(8) Uani 1 1 d . U .
H17A H 0.1215 -0.0067 0.4162 0.116 Uiso 1 1 calc R U .
H17B H 0.0131 0.0043 0.4037 0.116 Uiso 1 1 calc R U .
N18 N 0.006(3) 0.0362(10) 0.2895(18) 0.124(9) Uani 1 1 d . U .
H18A H 0.0103 0.0476 0.2491 0.149 Uiso 1 1 calc R U .
H18B H -0.0508 0.0354 0.3081 0.149 Uiso 1 1 calc R U .
C1 C 0.508(2) -0.0741(8) 0.7276(12) 0.058(4) Uani 1 1 d D U .
H1A H 0.4636 -0.0968 0.7124 0.069 Uiso 1 1 calc R U .
H1B H 0.5759 -0.0848 0.7322 0.069 Uiso 1 1 calc R U .
C2 C 0.480(2) -0.0599(8) 0.7983(11) 0.070(4) Uani 1 1 d D U .
H2A H 0.4123 -0.0486 0.7933 0.084 Uiso 1 1 calc R U .
H2B H 0.5248 -0.0374 0.8136 0.084 Uiso 1 1 calc R U .
C3 C 0.4838(19) -0.0924(9) 0.8551(16) 0.080(4) Uani 1 1 d D U .
C4 C 0.0396(16) -0.1235(7) 0.5913(13) 0.038(6) Uani 1 1 d . U .
C5 C -0.0860(18) 0.2340(8) 0.4503(13) 0.041(6) Uani 1 1 d . U .
C6 C 0.9537(19) 0.1798(9) 0.8334(17) 0.053(8) Uani 1 1 d . . .
C7 C 1.008(2) 0.0733(11) 0.7757(16) 0.068(9) Uani 1 1 d . . .
C8 C 0.428(2) 0.1944(9) 0.2470(14) 0.049(7) Uani 1 1 d . . .
C9 C 0.091(3) 0.0192(13) 0.325(2) 0.100(7) Uani 1 1 d . U .
O1W O 0.257(2) 0.1788(10) 1.0831(16) 0.139(11) Uiso 1 1 d . . .
O2W O 0.184(2) -0.0425(8) 0.6617(14) 0.115(9) Uiso 1 1 d . . .
O3W O 0.407(2) 0.1290(9) 1.0303(16) 0.106(10) Uiso 0.85 1 d . . P
O4W O 0.094(3) 0.3157(12) 0.544(2) 0.108(13) Uiso 0.65 1 d . . P
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sn Sn -0.6537 1.4246 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O25 W1 O4 98.0(6) . .
O25 W1 O11 100.2(6) . .
O4 W1 O11 93.4(6) . .
O25 W1 O6 102.1(6) . .
O4 W1 O6 91.9(6) . .
O11 W1 O6 156.1(5) . .
O25 W1 O39 94.4(6) . .
O4 W1 O39 167.3(5) . .
O11 W1 O39 87.3(5) . .
O6 W1 O39 82.5(5) . .
O25 W1 O17 172.0(5) . .
O4 W1 O17 87.2(5) . .
O11 W1 O17 73.3(5) . .
O6 W1 O17 83.7(5) . .
O39 W1 O17 80.9(5) . .
O49 W2 O8 102.1(6) . .
O49 W2 O51 100.3(7) . .
O8 W2 O51 93.6(6) . .
O49 W2 O10 101.7(6) . .
O8 W2 O10 90.0(6) . .
O51 W2 O10 156.4(6) . .
O49 W2 O43 96.9(6) . .
O8 W2 O43 160.7(6) . .
O51 W2 O43 86.1(6) . .
O10 W2 O43 82.9(6) . .
O49 W2 O14 171.9(6) . .
O8 W2 O14 82.6(5) . .
O51 W2 O14 72.6(5) . .
O10 W2 O14 84.7(5) . .
O43 W2 O14 78.9(5) . .
O7 W3 O19 101.9(7) . .
O7 W3 O51 100.1(6) . .
O19 W3 O51 93.5(6) . .
O7 W3 O9 101.2(6) . .
O19 W3 O9 89.4(6) . .
O51 W3 O9 157.4(6) . .
O7 W3 O22 96.0(7) . .
O19 W3 O22 161.8(6) . .
O51 W3 O22 86.6(6) . .
O9 W3 O22 83.8(6) . .
O7 W3 O14 172.0(6) . .
O19 W3 O14 83.2(5) . .
O51 W3 O14 73.2(5) . .
O9 W3 O14 84.9(5) . .
O22 W3 O14 79.4(5) . .
O1 W4 O40 102.5(7) . .
O1 W4 O47 101.6(6) . .
O40 W4 O47 96.1(6) . .
O1 W4 O11 99.9(6) . .
O40 W4 O11 91.3(6) . .
O47 W4 O11 155.1(5) . .
O1 W4 O50 91.8(6) . .
O40 W4 O50 165.3(6) . .
O47 W4 O50 84.2(5) . .
O11 W4 O50 82.7(5) . .
O1 W4 O17 169.7(6) . .
O40 W4 O17 84.1(6) . .
O47 W4 O17 85.3(5) . .
O11 W4 O17 71.8(5) . .
O50 W4 O17 81.3(5) . .
O13 W5 O23 100.7(7) . .
O13 W5 O15 99.9(6) . .
O23 W5 O15 94.9(6) . .
O13 W5 O6 102.4(6) . .
O23 W5 O6 91.5(5) . .
O15 W5 O6 155.2(6) . .
O13 W5 O52 92.6(6) . .
O23 W5 O52 166.0(6) . .
O15 W5 O52 86.8(5) . .
O6 W5 O52 81.4(5) . .
O13 W5 O16 169.4(6) . .
O23 W5 O16 87.6(5) . .
O15 W5 O16 72.7(5) . .
O6 W5 O16 83.6(5) . .
O52 W5 O16 79.6(5) . .
O44 W6 O50 101.5(6) . .
O44 W6 O9 102.0(6) . .
O50 W6 O9 91.7(5) . .
O44 W6 O30 97.6(6) . .
O50 W6 O30 93.3(6) . .
O9 W6 O30 158.4(5) . .
O44 W6 O18 95.7(6) . .
O50 W6 O18 162.7(5) . .
O9 W6 O18 83.5(5) . .
O30 W6 O18 85.5(6) . .
O44 W6 O26 170.0(6) . .
O50 W6 O26 83.8(5) . .
O9 W6 O26 86.2(5) . .
O30 W6 O26 73.5(5) . .
O18 W6 O26 79.4(5) . .
O24 W7 O36 101.0(6) . .
O24 W7 O34 102.5(6) . .
O36 W7 O34 87.7(5) . .
O24 W7 O41 98.8(6) . .
O36 W7 O41 93.2(5) . .
O34 W7 O41 158.1(5) . .
O24 W7 O23 97.3(6) . .
O36 W7 O23 161.4(6) . .
O34 W7 O23 84.9(5) . .
O41 W7 O23 87.4(5) . .
O24 W7 O20 170.8(5) . .
O36 W7 O20 84.3(5) . .
O34 W7 O20 85.2(5) . .
O41 W7 O20 73.2(5) . .
O23 W7 O20 78.1(5) . .
O46 W8 O35 101.3(6) . .
O46 W8 O2 102.7(6) . .
O35 W8 O2 91.6(6) . .
O46 W8 O12 99.5(6) . .
O35 W8 O12 91.4(6) . .
O2 W8 O12 156.6(5) . .
O46 W8 O8 97.2(6) . .
O35 W8 O8 161.4(5) . .
O2 W8 O8 86.0(5) . .
O12 W8 O8 83.8(6) . .
O46 W8 O5 172.7(6) . .
O35 W8 O5 80.3(5) . .
O2 W8 O5 84.3(5) . .
O12 W8 O5 73.2(5) . .
O8 W8 O5 81.1(5) . .
O29 W9 O21 101.9(6) . .
O29 W9 O10 101.2(6) . .
O21 W9 O10 93.0(6) . .
O29 W9 O41 97.3(6) . .
O21 W9 O41 92.1(6) . .
O10 W9 O41 159.4(5) . .
O29 W9 O45 96.2(6) . .
O21 W9 O45 161.9(5) . .
O10 W9 O45 82.6(6) . .
O41 W9 O45 86.4(5) . .
O29 W9 O20 170.1(6) . .
O21 W9 O20 82.6(5) . .
O10 W9 O20 87.3(5) . .
O41 W9 O20 73.6(5) . .
O45 W9 O20 79.6(5) . .
O38 W10 O55 100.1(6) . .
O38 W10 O2 102.0(6) . .
O55 W10 O2 94.9(6) . .
O38 W10 O15 100.3(6) . .
O55 W10 O15 89.7(6) . .
O2 W10 O15 156.0(5) . .
O38 W10 O21 95.8(6) . .
O55 W10 O21 163.6(5) . .
O2 W10 O21 85.7(6) . .
O15 W10 O21 83.4(6) . .
O38 W10 O16 171.0(6) . .
O55 W10 O16 83.0(5) . .
O2 W10 O16 86.0(5) . .
O15 W10 O16 71.2(5) . .
O21 W10 O16 80.7(5) . .
O48 W11 O37 100.6(6) . .
O48 W11 O30 98.9(6) . .
O37 W11 O30 92.7(6) . .
O48 W11 O34 102.8(6) . .
O37 W11 O34 86.9(6) . .
O30 W11 O34 158.0(5) . .
O48 W11 O4 97.7(6) . .
O37 W11 O4 161.2(6) . .
O30 W11 O4 89.0(6) . .
O34 W11 O4 84.5(6) . .
O48 W11 O26 171.3(6) . .
O37 W11 O26 84.1(5) . .
O30 W11 O26 73.4(5) . .
O34 W11 O26 84.6(5) . .
O4 W11 O26 78.4(5) . .
O28 W12 O3 100.9(6) . .
O28 W12 O12 101.9(6) . .
O3 W12 O12 92.2(6) . .
O28 W12 O47 99.4(6) . .
O3 W12 O47 91.9(5) . .
O12 W12 O47 157.1(5) . .
O28 W12 O19 95.5(6) . .
O3 W12 O19 163.6(6) . .
O12 W12 O19 85.2(6) . .
O47 W12 O19 84.6(5) . .
O28 W12 O5 175.4(6) . .
O3 W12 O5 81.3(5) . .
O12 W12 O5 73.9(5) . .
O47 W12 O5 84.5(5) . .
O19 W12 O5 82.4(5) . .
O31 W13 O56 103.3(7) . .
O31 W13 O54 102.5(7) . .
O56 W13 O54 92.8(6) . .
O31 W13 O37 100.9(7) . .
O56 W13 O37 87.7(6) . .
O54 W13 O37 155.7(6) . .
O31 W13 O36 101.1(7) . .
O56 W13 O36 155.0(6) . .
O54 W13 O36 87.3(6) . .
O37 W13 O36 82.2(5) . .
O31 W13 O53 174.5(7) . .
O56 W13 O53 73.2(5) . .
O54 W13 O53 73.8(5) . .
O37 W13 O53 83.2(5) . .
O36 W13 O53 82.9(5) . .
O33 W14 O45 102.9(6) . .
O33 W14 O43 104.0(7) . .
O45 W14 O43 89.6(6) . .
O33 W14 O42 99.8(7) . .
O45 W14 O42 157.0(6) . .
O43 W14 O42 88.5(6) . .
O33 W14 O54 97.6(6) . .
O45 W14 O54 88.0(6) . .
O43 W14 O54 158.3(6) . .
O42 W14 O54 85.4(6) . .
O33 W14 O53 167.7(6) . .
O45 W14 O53 85.1(5) . .
O43 W14 O53 85.3(5) . .
O42 W14 O53 72.0(5) . .
O54 W14 O53 73.1(5) . .
O32 W15 O22 103.4(7) . .
O32 W15 O18 102.8(6) . .
O22 W15 O18 89.0(6) . .
O32 W15 O42 101.0(6) . .
O22 W15 O42 88.8(6) . .
O18 W15 O42 155.9(6) . .
O32 W15 O56 99.4(6) . .
O22 W15 O56 157.1(6) . .
O18 W15 O56 87.5(6) . .
O42 W15 O56 85.3(6) . .
O32 W15 O53 169.0(6) . .
O22 W15 O53 84.8(5) . .
O18 W15 O53 84.4(5) . .
O42 W15 O53 71.6(5) . .
O56 W15 O53 72.4(5) . .
O3 Sn1 O39 158.8(5) . 3_656
O3 Sn1 O35 91.0(5) . .
O39 Sn1 O35 87.4(5) 3_656 .
O3 Sn1 O52 87.3(5) . 3_656
O39 Sn1 O52 86.6(5) 3_656 3_656
O35 Sn1 O52 158.9(5) . 3_656
O3 Sn1 C1 95.8(8) . .
O39 Sn1 C1 105.4(8) 3_656 .
O35 Sn1 C1 95.8(8) . .
O52 Sn1 C1 105.2(8) 3_656 .
O3 Sn1 O27 82.4(5) . .
O39 Sn1 O27 76.4(5) 3_656 .
O35 Sn1 O27 82.4(5) . .
O52 Sn1 O27 76.5(5) 3_656 .
C1 Sn1 O27 177.5(7) . .
O40 Cu1 O55 93.2(5) . 3_656
O40 Cu1 O52 87.4(6) . 3_656
O55 Cu1 O52 102.9(5) 3_656 3_656
O40 Cu1 O39 101.4(6) . .
O55 Cu1 O39 86.1(5) 3_656 .
O52 Cu1 O39 167.2(5) 3_656 .
O40 Cu1 O27 175.1(6) . 3_656
O55 Cu1 O27 91.1(5) 3_656 3_656
O52 Cu1 O27 94.1(5) 3_656 3_656
O39 Cu1 O27 76.4(5) . 3_656
O40 Cu1 O27 90.6(5) . .
O55 Cu1 O27 176.2(5) 3_656 .
O52 Cu1 O27 77.2(5) 3_656 .
O39 Cu1 O27 93.3(5) . .
O27 Cu1 O27 85.2(5) 3_656 .
O16 P1 O5 112.4(7) . .
O16 P1 O17 111.6(7) . .
O5 P1 O17 111.5(7) . .
O16 P1 O27 106.9(8) . .
O5 P1 O27 106.7(7) . .
O17 P1 O27 107.3(8) . .
O14 P2 O26 111.4(8) . .
O14 P2 O20 113.2(7) . .
O26 P2 O20 112.1(8) . .
O14 P2 O53 107.3(7) . .
O26 P2 O53 106.2(7) . .
O20 P2 O53 106.0(7) . .
W10 O2 W8 148.9(8) . .
W12 O3 Sn1 140.0(7) . .
W1 O4 W11 167.4(8) . .
P1 O5 W12 127.7(7) . .
P1 O5 W8 127.3(7) . .
W12 O5 W8 90.1(4) . .
W5 O6 W1 160.9(8) . .
W2 O8 W8 166.5(8) . .
W6 O9 W3 154.4(8) . .
W9 O10 W2 155.8(8) . .
W1 O11 W4 123.2(6) . .
W12 O12 W8 122.2(7) . .
P2 O14 W3 130.2(7) . .
P2 O14 W2 128.9(7) . .
W3 O14 W2 90.0(4) . .
W5 O15 W10 124.3(7) . .
P1 O16 W10 128.1(7) . .
P1 O16 W5 133.9(7) . .
W10 O16 W5 91.4(4) . .
P1 O17 W1 132.8(8) . .
P1 O17 W4 127.1(7) . .
W1 O17 W4 91.6(4) . .
W15 O18 W6 149.3(7) . .
W3 O19 W12 167.4(8) . .
P2 O20 W9 128.8(7) . .
P2 O20 W7 127.2(7) . .
W9 O20 W7 92.0(4) . .
W9 O21 W10 162.2(8) . .
W15 O22 W3 149.8(8) . .
W5 O23 W7 167.2(8) . .
P2 O26 W6 129.9(8) . .
P2 O26 W11 127.0(8) . .
W6 O26 W11 90.6(4) . .
P1 O27 Cu1 116.9(8) . 3_656
P1 O27 Cu1 118.6(8) . .
Cu1 O27 Cu1 94.8(5) 3_656 .
P1 O27 Sn1 125.8(7) . .
Cu1 O27 Sn1 97.7(5) 3_656 .
Cu1 O27 Sn1 96.7(6) . .
W11 O30 W6 122.3(6) . .
W11 O34 W7 148.1(8) . .
W8 O35 Sn1 141.8(7) . .
W7 O36 W13 152.2(7) . .
W11 O37 W13 152.7(8) . .
Sn1 O39 W1 120.3(6) 3_656 .
Sn1 O39 Cu1 109.4(6) 3_656 .
W1 O39 Cu1 126.0(6) . .
W4 O40 Cu1 133.5(8) . .
W7 O41 W9 121.1(6) . .
W14 O42 W15 123.4(7) . .
W14 O43 W2 149.1(8) . .
W14 O45 W9 148.9(7) . .
W4 O47 W12 147.2(7) . .
W6 O50 W4 163.3(7) . .
W2 O51 W3 123.2(7) . .
Sn1 O52 W5 121.4(6) 3_656 .
Sn1 O52 Cu1 109.4(6) 3_656 3_656
W5 O52 Cu1 125.4(6) . 3_656
P2 O53 W14 122.4(7) . .
P2 O53 W15 122.8(7) . .
W14 O53 W15 93.0(4) . .
P2 O53 W13 127.6(7) . .
W14 O53 W13 90.7(4) . .
W15 O53 W13 90.6(4) . .
W13 O54 W14 122.4(7) . .
W10 O55 Cu1 132.1(8) . 3_656
W13 O56 W15 123.7(7) . .
C4 N1 H1C 120.0 . .
C4 N1 H1D 120.0 . .
H1C N1 H1D 120.0 . .
C4 N2 H2C 120.0 . .
C4 N2 H2D 120.0 . .
H2C N2 H2D 120.0 . .
C4 N3 H3A 120.0 . .
C4 N3 H3B 120.0 . .
H3A N3 H3B 120.0 . .
C5 N4 H4A 120.0 . .
C5 N4 H4B 120.0 . .
H4A N4 H4B 120.0 . .
C5 N5 H5A 120.0 . .
C5 N5 H5B 120.0 . .
H5A N5 H5B 120.0 . .
C5 N6 H6A 120.0 . .
C5 N6 H6B 120.0 . .
H6A N6 H6B 120.0 . .
C6 N7 H7A 120.0 . .
C6 N7 H7B 120.0 . .
H7A N7 H7B 120.0 . .
C6 N8 H8A 120.0 . .
C6 N8 H8B 120.0 . .
H8A N8 H8B 120.0 . .
C6 N9 H9A 120.0 . .
C6 N9 H9B 120.0 . .
H9A N9 H9B 120.0 . .
C7 N10 H10A 120.0 . .
C7 N10 H10B 120.0 . .
H10A N10 H10B 120.0 . .
C7 N11 H11A 120.0 . .
C7 N11 H11B 120.0 . .
H11A N11 H11B 120.0 . .
C7 N12 H12A 120.0 . .
C7 N12 H12B 120.0 . .
H12A N12 H12B 120.0 . .
C8 N13 H13A 120.0 . .
C8 N13 H13B 120.0 . .
H13A N13 H13B 120.0 . .
C8 N14 H14A 120.0 . .
C8 N14 H14B 120.0 . .
H14A N14 H14B 120.0 . .
C8 N15 H15A 120.0 . .
C8 N15 H15B 120.0 . .
H15A N15 H15B 120.0 . .
C9 N16 H16A 120.0 . .
C9 N16 H16B 120.0 . .
H16A N16 H16B 120.0 . .
C9 N17 H17A 120.0 . .
C9 N17 H17B 120.0 . .
H17A N17 H17B 120.0 . .
C9 N18 H18A 120.0 . .
C9 N18 H18B 120.0 . .
H18A N18 H18B 120.0 . .
C2 C1 Sn1 115.0(17) . .
C2 C1 H1A 108.5 . .
Sn1 C1 H1A 108.5 . .
C2 C1 H1B 108.5 . .
Sn1 C1 H1B 108.5 . .
H1A C1 H1B 107.5 . .
C1 C2 C3 116(2) . .
C1 C2 H2A 108.3 . .
C3 C2 H2A 108.3 . .
C1 C2 H2B 108.3 . .
C3 C2 H2B 108.3 . .
H2A C2 H2B 107.4 . .
O58 C3 O57 130(3) . .
O58 C3 C2 112(2) . .
O57 C3 C2 116(3) . .
N2 C4 N1 121(2) . .
N2 C4 N3 121(2) . .
N1 C4 N3 118(2) . .
N5 C5 N4 123(2) . .
N5 C5 N6 121(3) . .
N4 C5 N6 116(2) . .
N8 C6 N9 121(3) . .
N8 C6 N7 121(3) . .
N9 C6 N7 118(2) . .
N12 C7 N11 122(3) . .
N12 C7 N10 119(3) . .
N11 C7 N10 118(3) . .
N14 C8 N15 124(3) . .
N14 C8 N13 119(2) . .
N15 C8 N13 117(3) . .
N16 C9 N17 124(4) . .
N16 C9 N18 123(4) . .
N17 C9 N18 113(4) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
W1 O25 1.701(14) .
W1 O4 1.842(12) .
W1 O11 1.878(12) .
W1 O6 1.914(12) .
W1 O39 2.080(12) .
W1 O17 2.353(13) .
W2 O49 1.719(14) .
W2 O8 1.815(13) .
W2 O51 1.902(14) .
W2 O10 1.916(14) .
W2 O43 2.011(13) .
W2 O14 2.391(12) .
W3 O7 1.724(14) .
W3 O19 1.821(13) .
W3 O51 1.916(13) .
W3 O9 1.917(13) .
W3 O22 1.991(14) .
W3 O14 2.357(13) .
W4 O1 1.705(13) .
W4 O40 1.797(15) .
W4 O47 1.881(12) .
W4 O11 1.963(12) .
W4 O50 2.066(12) .
W4 O17 2.360(12) .
W5 O13 1.704(13) .
W5 O23 1.835(12) .
W5 O15 1.854(12) .
W5 O6 1.894(12) .
W5 O52 2.076(12) .
W5 O16 2.361(12) .
W6 O44 1.708(13) .
W6 O50 1.811(12) .
W6 O9 1.867(14) .
W6 O30 1.955(14) .
W6 O18 2.010(13) .
W6 O26 2.344(13) .
W7 O24 1.711(14) .
W7 O36 1.854(13) .
W7 O34 1.903(13) .
W7 O41 1.924(13) .
W7 O23 1.949(12) .
W7 O20 2.358(13) .
W8 O46 1.704(13) .
W8 O35 1.800(12) .
W8 O2 1.916(13) .
W8 O12 1.925(13) .
W8 O8 1.996(13) .
W8 O5 2.383(12) .
W9 O29 1.704(13) .
W9 O21 1.837(13) .
W9 O10 1.858(14) .
W9 O41 1.946(14) .
W9 O45 2.020(13) .
W9 O20 2.326(12) .
W10 O38 1.713(13) .
W10 O55 1.803(14) .
W10 O2 1.868(14) .
W10 O15 1.962(13) .
W10 O21 2.017(12) .
W10 O16 2.355(12) .
W11 O48 1.683(14) .
W11 O37 1.871(14) .
W11 O30 1.888(13) .
W11 O34 1.891(12) .
W11 O4 1.942(12) .
W11 O26 2.392(14) .
W12 O28 1.684(13) .
W12 O3 1.819(13) .
W12 O12 1.912(13) .
W12 O47 1.929(12) .
W12 O19 1.986(12) .
W12 O5 2.364(13) .
W13 O31 1.704(15) .
W13 O56 1.876(14) .
W13 O54 1.883(13) .
W13 O37 1.947(14) .
W13 O36 1.957(12) .
W13 O53 2.396(13) .
W14 O33 1.729(13) .
W14 O45 1.841(13) .
W14 O43 1.849(14) .
W14 O42 1.943(13) .
W14 O54 1.978(14) .
W14 O53 2.360(12) .
W15 O32 1.703(15) .
W15 O22 1.857(14) .
W15 O18 1.860(12) .
W15 O42 1.954(14) .
W15 O56 1.965(16) .
W15 O53 2.370(12) .
Sn1 O3 2.056(13) .
Sn1 O39 2.060(13) 3_656
Sn1 O35 2.064(13) .
Sn1 O52 2.065(13) 3_656
Sn1 C1 2.12(3) .
Sn1 O27 2.290(14) .
Cu1 O40 2.005(15) .
Cu1 O55 2.018(14) 3_656
Cu1 O52 2.085(12) 3_656
Cu1 O39 2.117(13) .
Cu1 O27 2.237(14) 3_656
Cu1 O27 2.241(15) .
P1 O16 1.515(13) .
P1 O5 1.521(13) .
P1 O17 1.543(13) .
P1 O27 1.619(15) .
P2 O14 1.521(14) .
P2 O26 1.522(13) .
P2 O20 1.536(13) .
P2 O53 1.592(13) .
O27 Cu1 2.237(14) 3_656
O39 Sn1 2.060(13) 3_656
O52 Sn1 2.065(13) 3_656
O52 Cu1 2.085(12) 3_656
O55 Cu1 2.018(14) 3_656
O57 C3 1.292(10) .
O58 C3 1.277(10) .
N1 C4 1.32(3) .
N1 H1C 0.8600 .
N1 H1D 0.8600 .
N2 C4 1.31(3) .
N2 H2C 0.8600 .
N2 H2D 0.8600 .
N3 C4 1.34(3) .
N3 H3A 0.8600 .
N3 H3B 0.8600 .
N4 C5 1.28(3) .
N4 H4A 0.8600 .
N4 H4B 0.8600 .
N5 C5 1.27(3) .
N5 H5A 0.8600 .
N5 H5B 0.8600 .
N6 C5 1.33(3) .
N6 H6A 0.8600 .
N6 H6B 0.8600 .
N7 C6 1.34(4) .
N7 H7A 0.8600 .
N7 H7B 0.8600 .
N8 C6 1.24(3) .
N8 H8A 0.8600 .
N8 H8B 0.8600 .
N9 C6 1.29(3) .
N9 H9A 0.8600 .
N9 H9B 0.8600 .
N10 C7 1.33(3) .
N10 H10A 0.8600 .
N10 H10B 0.8600 .
N11 C7 1.31(4) .
N11 H11A 0.8600 .
N11 H11B 0.8600 .
N12 C7 1.30(3) .
N12 H12A 0.8600 .
N12 H12B 0.8600 .
N13 C8 1.37(3) .
N13 H13A 0.8600 .
N13 H13B 0.8600 .
N14 C8 1.28(3) .
N14 H14A 0.8600 .
N14 H14B 0.8600 .
N15 C8 1.33(4) .
N15 H15A 0.8600 .
N15 H15B 0.8600 .
N16 C9 1.30(4) .
N16 H16A 0.8600 .
N16 H16B 0.8600 .
N17 C9 1.37(4) .
N17 H17A 0.8600 .
N17 H17B 0.8600 .
N18 C9 1.39(4) .
N18 H18A 0.8600 .
N18 H18B 0.8600 .
C1 C2 1.496(10) .
C1 H1A 0.9700 .
C1 H1B 0.9700 .
C2 C3 1.508(10) .
C2 H2A 0.9700 .
C2 H2B 0.9700 .
loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_site_symmetry_A
N1 H1C O11 0.86 2.10 2.94(2) 163.3 3_556
N1 H1D O33 0.86 2.02 2.88(3) 177.4 2_546
N2 H2C O1 0.86 2.18 3.04(2) 172.3 3_556
N2 H2D O15 0.86 2.09 2.92(2) 161.5 3_656
N3 H3A O13 0.86 2.22 3.07(2) 169.5 3_656
N3 H3B O42 0.86 2.15 2.98(2) 162.1 2_546
N4 H4A O43 0.86 2.21 3.06(3) 167.9 4_565
N4 H4B O30 0.86 1.98 2.82(2) 166.6 .
N5 H5A O22 0.86 2.12 2.90(3) 149.0 4_565
N5 H5A O51 0.86 2.59 3.23(3) 131.9 4_565
N5 H5B O24 0.86 2.14 2.97(3) 162.4 1_455
N6 H6A O41 0.86 2.08 2.91(3) 164.5 1_455
N6 H6B O44 0.86 2.04 2.89(2) 171.1 .
N7 H7A O29 0.86 2.32 3.12(3) 155.8 .
N7 H7B O7 0.86 2.58 3.32(3) 144.5 1_655
N8 H8B O29 0.86 2.55 3.31(4) 148.1 .
N8 H8B O10 0.86 2.64 3.34(3) 139.2 .
N9 H9A O31 0.86 2.27 3.13(3) 171.5 4_666
N9 H9B O7 0.86 2.22 3.05(3) 162.4 1_655
N10 H10B O38 0.86 2.37 3.10(3) 142.9 .
N10 H10B O2 0.86 2.64 3.38(3) 144.2 .
N11 H11A O47 0.86 2.28 3.10(3) 157.9 1_655
N11 H11B O38 0.86 2.13 2.92(3) 152.5 .
N12 H12A O28 0.86 2.21 3.01(3) 153.6 1_655
N13 H13A O48 0.86 2.34 3.11(3) 148.6 .
N13 H13A O33 0.86 2.64 3.08(3) 112.8 4_565
N13 H13B O1W 0.86 2.54 3.31(4) 148.3 1_554
N13 H13B O45 0.86 2.59 3.22(3) 130.7 4_565
N14 H14A O32 0.86 2.21 3.00(3) 153.0 4_665
N14 H14B O34 0.86 2.35 3.11(3) 146.6 .
N15 H15A O32 0.86 2.44 3.16(4) 142.2 4_665
N15 H15B O1W 0.86 2.54 3.31(4) 149.5 1_554
N16 H16A O55 0.86 2.41 3.16(3) 144.6 3_656
N16 H16A O35 0.86 2.52 3.19(3) 136.0 3_656
N17 H17A O55 0.86 2.36 3.11(3) 144.9 3_656
N17 H17B O1 0.86 2.43 3.03(3) 127.3 3_556
N18 H18B O2W 0.86 1.91 2.76(4) 169.0 3_556
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_4
O38 W10 O2 W8 -130.5(14) .
O55 W10 O2 W8 -29.0(15) .
O15 W10 O2 W8 71(2) .
O21 W10 O2 W8 134.6(14) .
O16 W10 O2 W8 53.6(14) .
O28 W12 O3 Sn1 -136.0(10) .
O12 W12 O3 Sn1 -33.5(11) .
O47 W12 O3 Sn1 124.0(10) .
O19 W12 O3 Sn1 47(2) .
O5 W12 O3 Sn1 39.9(10) .
O25 W1 O4 W11 -84(4) .
O11 W1 O4 W11 175(4) .
O6 W1 O4 W11 18(4) .
O39 W1 O4 W11 82(5) .
O17 W1 O4 W11 102(4) .
O16 P1 O5 W12 -179.5(8) .
O17 P1 O5 W12 54.3(11) .
O27 P1 O5 W12 -62.6(10) .
O16 P1 O5 W8 -53.2(11) .
O17 P1 O5 W8 -179.4(8) .
O27 P1 O5 W8 63.7(10) .
O13 W5 O6 W1 149(2) .
O23 W5 O6 W1 -109(2) .
O15 W5 O6 W1 -4(3) .
O52 W5 O6 W1 58(2) .
O16 W5 O6 W1 -22(2) .
O49 W2 O8 W8 -88(3) .
O51 W2 O8 W8 171(3) .
O10 W2 O8 W8 14(3) .
O43 W2 O8 W8 82(4) .
O14 W2 O8 W8 99(3) .
O44 W6 O9 W3 -136.7(17) .
O50 W6 O9 W3 121.1(17) .
O30 W6 O9 W3 18(3) .
O18 W6 O9 W3 -42.3(17) .
O26 W6 O9 W3 37.5(17) .
O29 W9 O10 W2 141(2) .
O21 W9 O10 W2 -117(2) .
O41 W9 O10 W2 -13(3) .
O45 W9 O10 W2 46(2) .
O20 W9 O10 W2 -34(2) .
O25 W1 O11 W4 178.3(8) .
O4 W1 O11 W4 -83.0(8) .
O6 W1 O11 W4 19.7(18) .
O39 W1 O11 W4 84.3(8) .
O17 W1 O11 W4 3.0(7) .
O26 P2 O14 W3 -50.2(11) .
O20 P2 O14 W3 -177.6(8) .
O53 P2 O14 W3 65.7(10) .
O26 P2 O14 W2 177.0(8) .
O20 P2 O14 W2 49.5(11) .
O53 P2 O14 W2 -67.2(10) .
O13 W5 O15 W10 -178.7(8) .
O23 W5 O15 W10 79.5(8) .
O6 W5 O15 W10 -25.0(18) .
O52 W5 O15 W10 -86.6(8) .
O16 W5 O15 W10 -6.5(7) .
O5 P1 O16 W10 50.4(11) .
O17 P1 O16 W10 176.6(8) .
O27 P1 O16 W10 -66.3(10) .
O5 P1 O16 W5 -166.7(9) .
O17 P1 O16 W5 -40.5(12) .
O27 P1 O16 W5 76.6(11) .
O16 P1 O17 W1 41.9(12) .
O5 P1 O17 W1 168.6(9) .
O27 P1 O17 W1 -74.9(11) .
O16 P1 O17 W4 -179.7(8) .
O5 P1 O17 W4 -53.0(11) .
O27 P1 O17 W4 63.5(10) .
O32 W15 O18 W6 -127.1(15) .
O22 W15 O18 W6 -23.6(15) .
O42 W15 O18 W6 61(2) .
O56 W15 O18 W6 133.8(15) .
O53 W15 O18 W6 61.2(14) .
O7 W3 O19 W12 96(4) .
O51 W3 O19 W12 -163(4) .
O9 W3 O19 W12 -5(4) .
O22 W3 O19 W12 -73(4) .
O14 W3 O19 W12 -90(4) .
O14 P2 O20 W9 -47.7(11) .
O26 P2 O20 W9 -174.8(8) .
O53 P2 O20 W9 69.7(10) .
O14 P2 O20 W7 -179.7(7) .
O26 P2 O20 W7 53.3(11) .
O53 P2 O20 W7 -62.3(10) .
O29 W9 O21 W10 84(2) .
O10 W9 O21 W10 -18(2) .
O41 W9 O21 W10 -178(2) .
O45 W9 O21 W10 -94(3) .
O20 W9 O21 W10 -105(2) .
O32 W15 O22 W3 125.5(16) .
O18 W15 O22 W3 22.5(16) .
O42 W15 O22 W3 -133.5(17) .
O56 W15 O22 W3 -59(3) .
O53 W15 O22 W3 -61.9(16) .
O13 W5 O23 W7 82(4) .
O15 W5 O23 W7 -177(4) .
O6 W5 O23 W7 -21(4) .
O52 W5 O23 W7 -81(5) .
O16 W5 O23 W7 -105(4) .
O14 P2 O26 W6 48.6(11) .
O20 P2 O26 W6 176.7(8) .
O53 P2 O26 W6 -67.8(11) .
O14 P2 O26 W11 178.8(8) .
O20 P2 O26 W11 -53.1(11) .
O53 P2 O26 W11 62.3(10) .
O16 P1 O27 Cu1 -3.7(10) 3_656
O5 P1 O27 Cu1 -124.2(8) 3_656
O17 P1 O27 Cu1 116.2(8) 3_656
O16 P1 O27 Cu1 -116.3(8) .
O5 P1 O27 Cu1 123.2(8) .
O17 P1 O27 Cu1 3.6(10) .
O16 P1 O27 Sn1 119.8(9) .
O5 P1 O27 Sn1 -0.7(12) .
O17 P1 O27 Sn1 -120.4(9) .
O48 W11 O30 W6 171.2(8) .
O37 W11 O30 W6 -87.6(8) .
O34 W11 O30 W6 1(2) .
O4 W11 O30 W6 73.6(8) .
O26 W11 O30 W6 -4.6(7) .
O48 W11 O34 W7 127.3(13) .
O37 W11 O34 W7 27.2(13) .
O30 W11 O34 W7 -63(2) .
O4 W11 O34 W7 -136.0(14) .
O26 W11 O34 W7 -57.2(13) .
O46 W8 O35 Sn1 132.6(12) .
O2 W8 O35 Sn1 -124.1(12) .
O12 W8 O35 Sn1 32.6(12) .
O8 W8 O35 Sn1 -42(3) .
O5 W8 O35 Sn1 -40.1(11) .
O24 W7 O36 W13 134.1(17) .
O34 W7 O36 W13 31.8(17) .
O41 W7 O36 W13 -126.3(17) .
O23 W7 O36 W13 -35(3) .
O20 W7 O36 W13 -53.6(17) .
O48 W11 O37 W13 -136.0(17) .
O30 W11 O37 W13 124.4(17) .
O34 W11 O37 W13 -33.5(17) .
O4 W11 O37 W13 29(3) .
O26 W11 O37 W13 51.4(17) .
O1 W4 O40 Cu1 144.1(10) .
O47 W4 O40 Cu1 -112.5(10) .
O11 W4 O40 Cu1 43.6(10) .
O50 W4 O40 Cu1 -22(3) .
O17 W4 O40 Cu1 -27.9(9) .
O33 W14 O43 W2 -125.5(14) .
O45 W14 O43 W2 -22.4(14) .
O42 W14 O43 W2 134.7(14) .
O54 W14 O43 W2 61(2) .
O53 W14 O43 W2 62.7(14) .
O33 W14 O45 W9 129.7(14) .
O43 W14 O45 W9 25.4(14) .
O42 W14 O45 W9 -60(2) .
O54 W14 O45 W9 -133.1(14) .
O53 W14 O45 W9 -59.9(14) .
O1 W4 O47 W12 130.6(13) .
O40 W4 O47 W12 26.5(14) .
O11 W4 O47 W12 -80.1(19) .
O50 W4 O47 W12 -138.8(14) .
O17 W4 O47 W12 -57.0(13) .
O44 W6 O50 W4 -95(2) .
O9 W6 O50 W4 7(2) .
O30 W6 O50 W4 166(2) .
O18 W6 O50 W4 81(3) .
O26 W6 O50 W4 93(2) .
O14 P2 O53 W14 60.3(9) .
O26 P2 O53 W14 179.5(8) .
O20 P2 O53 W14 -61.0(10) .
O14 P2 O53 W15 -58.6(9) .
O26 P2 O53 W15 60.6(10) .
O20 P2 O53 W15 -179.9(7) .
O14 P2 O53 W13 -179.4(7) .
O26 P2 O53 W13 -60.2(10) .
O20 P2 O53 W13 59.3(10) .
O31 W13 O54 W14 172.3(9) .
O56 W13 O54 W14 68.0(9) .
O37 W13 O54 W14 -23(2) .
O36 W13 O54 W14 -86.9(9) .
O53 W13 O54 W14 -3.6(7) .
O38 W10 O55 Cu1 -143.7(10) 3_656
O2 W10 O55 Cu1 113.1(10) 3_656
O15 W10 O55 Cu1 -43.3(10) 3_656
O21 W10 O55 Cu1 22(3) 3_656
O16 W10 O55 Cu1 27.7(9) 3_656
O31 W13 O56 W15 -171.9(9) .
O54 W13 O56 W15 -68.4(9) .
O37 W13 O56 W15 87.4(9) .
O36 W13 O56 W15 21.2(19) .
O53 W13 O56 W15 3.7(7) .
Sn1 C1 C2 C3 179.0(19) .
C1 C2 C3 O58 86(4) .
C1 C2 C3 O57 -83(4) .
loop_
_platon_squeeze_void_nr
_platon_squeeze_void_average_x
_platon_squeeze_void_average_y
_platon_squeeze_void_average_z
_platon_squeeze_void_volume
_platon_squeeze_void_count_electrons
1 -0.007 0.000 0.000 722.8 266.7
2 -0.002 0.500 0.500 722.7 270.0
